Resonant Photonic States in Coupled Heterostructure Photonic Crystal Waveguides
© The Author(s) 2010
Received: 5 October 2009
Accepted: 28 January 2010
Published: 9 February 2010
Skip to main content
© The Author(s) 2010
Received: 5 October 2009
Accepted: 28 January 2010
Published: 9 February 2010
In this paper, we study the photonic resonance states and transmission spectra of coupled waveguides made from heterostructure photonic crystals. We consider photonic crystal waveguides made from three photonic crystals A, B and C, where the waveguide heterostructure is denoted as B/A/C/A/B. Due to the band structure engineering, light is confined within crystal A, which thus act as waveguides. Here, photonic crystal C is taken as a nonlinear photonic crystal, which has a band gap that may be modified by applying a pump laser. We have found that the number of bound states within the waveguides depends on the width and well depth of photonic crystal A. It has also been found that when both waveguides are far away from each other, the energies of bound photons in each of the waveguides are degenerate. However, when they are brought close to each other, the degeneracy of the bound states is removed due to the coupling between them, which causes these states to split into pairs. We have also investigated the effect of the pump field on photonic crystal C. We have shown that by applying a pump field, the system may be switched between a double waveguide to a single waveguide, which effectively turns on or off the coupling between degenerate states. This reveals interesting results that can be applied to develop new types of nanophotonic devices such as nano-switches and nano-transistors.
There has been a great deal of interest in photonic crystals [1, 2] due to their ability to manipulate the propagation of light in the same way that semiconductor materials are able to control the propagation of electrons. Photonic crystals are materials with a dielectric constant that varies periodically in one, two or three spatial dimensions, due to which a photonic band gap forms in the structure’s photonic dispersion relation. Significant effort has been devoted to the development of new photonic devices made from photonic crystals. Two promising classes of these materials are photonic crystal heterostructures  and nonlinear photonic crystals [4–14].
Photonic crystal heterostructures are formed by joining two or more photonic crystals into a single structure, which gives the heterostructure a more complex band structure than that of a raw photonic crystal . Photonic crystal heterostructures have been successfully used to develop devices such as high-quality resonant cavities , low-loss waveguides  and high-efficiency add-drop filters . Nonlinear photonic crystals possess a PBG that can be shifted, which makes these materials ideal for developing optical switching devices. Recently, optical switching mechanisms due to nonlinear Kerr effects in photonic crystals have been studied both theoretically [4–9] and experimentally [10–14].
Here, we study the photonic resonance states and transmission spectra in coupled waveguides made from heterostructure photonic crystals. Waveguides made by embedding a high refractive index material into a low index material have been widely studied . Some work has also been done on photonic crystal waveguides formed by doping a dielectric material into a photonic crystal. For example, McGurn  and Sinha  have studied co-directional coupling between two photonic crystal waveguides. Faraon et al.  have studied theoretically and experimentally the coupling between photonic crystal waveguides.
In this paper, we consider two linear photonic crystals A and B and a nonlinear photonic crystal C and arrange them as B/A/C/A/B to form the waveguide heterostructure. Crystal parameters for A, B and C are chosen so that the upper band edge of crystal A lies within the band gaps of crystals B and C. Due to this band structure engineering, light is confined within crystal A, which thus act as waveguides. In the confinement direction of the waveguide, photons will occupy discrete quantized states within photonic crystal A, which appear as photonic quantum wells (PQWs). This so-called photonic confinement effect has been demonstrated both theoretically [22–24] and experimentally [25, 26] for various types of PQW systems, analogous to the electronic confinement effect that occurs in semiconductor quantum wells. It has been shown that the phenomenon of resonant tunneling will occur for a PQW with sufficiently thin photonic barriers, whereby an incident photon possessing an energy matching a resonant state of the PQW will undergo perfect transmission through both barriers [22, 23]. Because of this, resonant states appear as sharp peaks approaching unity in the transmission spectrum of a PQW [22–26].
Using the transfer matrix method [22, 24, 27], we have determined the energies of bound photons within the coupled waveguides and calculated the transmission coefficient of the system in the direction of photon confinement. We have found that the number of bound states within the waveguides depends on the width and the well depth of the photonic wells. It has also been found that when both waveguides are far away from each other (or equivalently, the width of photonic crystal C is large), the energies of bound photons within the waveguides are degenerate. However, when the waveguides are brought close to each other, the degeneracy of the bound states is removed due to the coupling between them, which causes these states to split into symmetric and anti-symmetric pairs. We have also investigated the effect of the nonlinearity of photonic crystal C. By applying a pump laser, the photonic band gap of crystal C changes due to the Kerr effect . This change in band structure effectively modifies the energy barrier separating the waveguides, which in turn changes the splitting energy of the coupler. In other words, the energies of the couplers can be switched on and off by applying the pump laser. This reveals interesting results that can be applied to develop new types of nanophotonic devices such as nano-switches and nano-transistors [4–14].
In Eq. (1),k i is the Bloch wave vector, L i is the lattice constant, n s,i and n b,i are the indices of refraction of the spheres and background materials, respectively, a i and b i are the radius of the spheres and the distance between the spheres, respectively, and ε k is the photon energy. Although the isotropic band structure model employed here is an idealization, it leads to qualitatively correct physics and has been shown to exhibit many features of observed and simulated band structures for 3-D photonic crystals [28, 29].
Here, we choose crystal parameters such that the upper band edges of photonic crystals B and C are almost equal, and the upper band edge of photonic crystal A is below that of B and C, but not so far as to form a deep photonic well. This is done to ensure that the photonic wells formed within crystal A are shallow enough so that the shift in the band gap of crystal C will be great enough to eliminate the central photonic barrier. Thus, we can switch the system between a double waveguide and single, wider waveguide by applying a pump field.
It is considered that light in the form of transverse electric waves is incident upon the waveguide heterostructure in the direction of photon confinement. The transmission coefficient of the heterostructure is calculated for the confinement direction using the transfer matrix method , which matches the electric field and its first derivative at the interfaces between adjacent photonic crystal layers in order to relate the incident and reflected amplitudes in each layer via transfer matrix equation. The transfer matrix method is ideal for our simulations, because we are considering isotropic photonic crystals, and we are only concerned with light propagation along the direction of photon confinement. In principle, a photonic waveguide does not allow transmission through the outer photonic barriers, but here we allow for transmission to occur by choosing sufficiently thin outer photonic barriers that permit photonic tunneling to occur. We do this in order to study the resonant tunneling effect that occurs as a result, whereby the behavior of the bound photonic states in the waveguide can be studied from its transmission spectra. The energies of the bound states are not affected by the thickness of the outer photonic barriers, so this has no effect on energies of the bound states within the waveguides or their coupling strength. Using the dispersion relation given in Eq. (1), the transmission coefficient was obtained as a function of the incident photon energy and was plotted over the range of energies between the upper band edges of photonic crystals A and B in order to find the resonant states of the system. The transmission spectra were studied for instances when the pump field is on or off in order to observe the switching effect produced.
We consider a coupled heterostructure photonic crystal waveguide consisting of crystals A, B and C arranged as B/A/C/A/B. For these crystals, their specific 3-D lattice structures are not be specified, as the isotropic band structure model employed here is independent of the type of lattice considered. Photonic crystals A, B and C each have a dielectric background material consisting of titania (TiO2), such that n s,A = n s,B = n s,C = 2.5 [30, 31]. The spheres in crystals A and B are taken to be filled with air n b,A = n b,B = 1.00, whereas the dielectric spheres in crystal C are made of polystyrene, with n o = 1.59 and n nL = 1.14 × 10−12 cm2/W . We choose polystyrene as our nonlinear dielectric material due to its strong and fast Kerr nonlinear optical response [9, 14]. Since the third-order nonlinear susceptibility of titania is on the order of 10−15 cm2/W , photonic crystals A and B are considered to be linear in our simulations. The radii of the spheres in all three photonic crystals were taken as a A = a B = a C = 125 nm, and the lattice constants for each crystal were taken as L A = 520 nm, L B = 510 nm and L C = 435 nm. The upper photonic band edges of photonic crystals A and B were calculated from Eq. (1) as 0.79273 eV and 0.81830 eV, respectively. When the pump field is off, the upper photonic band edge of photonic crystal C is found to be 0.82349 eV. Transmission spectra of the heterostructure are plotted between the upper band edges of photonic crystals A and B in order to study the resonant photonic states in the waveguide heterostructure.
Here, we have considered coupled heterostructure photonic crystal waveguides made from two photonic crystals A and B and another nonlinear photonic crystal C, where the heterostructure is denoted as B/A/C/A/B. Due to the band structure engineering, light is confined within photonic crystal A by crystals B and C, causing two waveguides to form in crystal A. Using the transfer matrix method, we have studied the resonant photonic states within the waveguides by calculating the transmission coefficient of the system in the direction of photon confinement. We have found that the number of bound photonic states within the waveguides can be controlled by varying the width and/or well depth of photonic crystal A. It was also found that when the waveguides are far away from each other, the energies of the bound photons are degenerate. However, by bringing the waveguides near one another, the degeneracy of the bound states is removed due to coupling between them, causing these states to undergo a twofold energy-splitting effect. Here, we have also investigated the nonlinearity of photonic crystal C. By applying a pump laser, the photonic band gap of crystal C changes due to the Kerr nonlinearity. The change in band structure causes the central photonic barrier to disappear, switching the system between single and double waveguide states. Essentially, this means that the energy-splitting effect can be turned off by applying a pump laser. It is expected that these results can be applied to develop new types of nanophotonic switching devices.
This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.